, B. Gligorijevićb
, B. Katavićb
, B. Nedićc
, D. Džunićc
a UniversityofBelgrade,FacultyofMechanicalEngineering,Belgrade,Serbia, b InstituteGoša,Belgrade,Serbia,
Keywords: Abrasivewear Scratchtest Hardfacing
A B S T R A C T
Abrasive wear is oneof the most common types of wear, which makes abrasive wear resistance very important in many industries. The hardfacing is considered as useful and economical way to improve the performanceofcomponentssubmittedtosevereabrasivewearconditions, with wide range of applicable filler materials. The abrasive wear resistance ofthethreedifferenthardfaced coatings(two iron‐based and one WC‐based), which were intended to be used for reparation of the impact plates of the ventilation mill, was investigated and compared. Abrasiveweartestswerecarried‐outbyusingthescratchtesterunderthe dryconditions.Threenormalloadsof10,50and100Nandtheconstant slidingspeedof4mm/swereused.Scratchtestwaschosenasarelatively easyandquicktestmethod.Wearmechanismanalysisshowedsignificant influenceofthehardfacedcoatingsstructure,which,alongwithhardness, hasdeterminedcoatingsabrasivewearresistance.
© Published by Faculty of Engineering Corresponding author:
TribologyLaboratory,Universityof Belgrade,FacultyofMechanical Engineering,KraljiceMarije16, 11120Belgrade35,Serbia E‐mail:firstname.lastname@example.org
More than % of all wear‐related failures of industrial equipment are caused by abrasive wear [ ]. The estimated costs of abrasive wear are between and % of the gross national product of an industrialized nation [ ]. For these reasons, the abrasive wear resistance is a subject of great importance in many industries, such as agriculture, mining, mineral processing etc.
(ardfacing could be defined as coating deposition process in which a wear resistant,
usually harder, material is deposited on the surface of a component by some of the welding techniques . )n most cases, hardfacing is used for controlling abrasive and erosive wear, like in mining, crushing and grinding, and agriculture industries buckets, bucket teeth, mill hammers, ball mills, digging tools, conveyer screws, etc. [ , ] . (ardfacing is also used to control combinations of wear and corrosion, as encountered by mud seals, plows, knives in the food processing industry, pumps handling corrosive liquids, or slurries [ ]. The hardfacing is considered as economical way to improve the
performance of components submitted to severe wear conditions, with wide range of applicable filler materials [ , ].
The iron‐based filler materials have drawn much attention due to their low cost and good resistance to abrasion in the hardfaced condition. (owever, their use is limited in applications where high impact loading is present, i.e. high‐stress or gouging abrasion [ ]. For this reason, efforts are being made towards the improvement of their impact and other properties [ ]. The progress is achieved mostly by modifying the hardfaced coating’s structure. Taking into account their low price and improved properties, the resistance to abrasive wear of the iron‐based hardfaced coatings is normally tested against the resistance of proven, but more expensive materials, such as WC‐based hardfaced coatings.
Abrasive wear has been defined as wear by displacement of material from surfaces in relative motion caused by the presence of hard particles either between the surfaces or embedded in one of them, or by the presence of hard protuberances on one or both of the surfaces [ ]. The second part of this definition corresponds to pure two‐body abrasion, where tested material slides against harder and rougher counter face material, while the first part corresponds to the three‐ and two‐body abrasion, respectively. Another interesting example of two‐body abrasion is the abrasive erosion, which is the special case of erosive wear. Abrasive erosion has been defined as erosive wear in which the loss of material from a solid surface is due to relative motion of solid particles which are entrained in a fluid, moving nearly parallel to a solid surface [ ]. Scratch test offers a possibility for comparison of different materials relatively easy and in short period of time, with good reproducibility [ ]. )n single‐pass scratch test a stylus which tip is made of hard material slide over the test sample producing a single scratch, which seems to be appropriate simulation of the two‐body abrasion.
)n this study, the abrasive wear resistance of the three different hardfaced coatings two iron‐ based and one WC‐based was investigated and compared.
The filler materials coating materials were manufactured by Castolin Eutectic Co. Ltd, Vienna. Their nominal chemical composition is shown in Table . The iron‐based filler materials basic covered electrodes were deposited by using the shielded metal arc welding SMAW process. The WC‐based filler material was deposited by oxy‐fuel gas welding OFW process. The substrate material was the hot‐rolled S J G steel.
Table1. Coatings composition, process and hardness.
Coating Nominal chemical composition (ardfacing process (ardness (V
T WC‐Ni‐Cr‐Si‐B OFW
All coatings were deposited by hardfacing in a single pass one layer . The substrate preparation and hardfacing procedures deposition parameters are described elsewhere [ , ]. The measurements of near‐ surface hardness are performed on the cross‐ section of hardfaced samples by Vickers indenter (V , and presented in Table .
The samples for structure characterization are obtained by cutting the hardfaced materials perpendicular to coatings surface. The obtained cross‐sections are ground with SiC abrasive papers down to P and polished with alumina suspensions down to μm. The polished surfaces are analyzed by using the scanning electron microscope SEM equipped with energy dispersive system EDS . The SEM‐EDS analysis was performed at University of Belgrade, Faculty of Mining and Geology by using the JEOL JSM– LV SEM connected with the )NCA energy dispersion X‐ray analysis unit. The electron acceleration voltage of kV and the tungsten filament were used. Before SEM‐EDS analysis was performed, polished surfaces were nm gold coated in a vacuum chamber by use of a sputter coater device.
Fig.1. The structures SEM of: a , b and c T hardfaced coating; back‐scattered electron images.
The material during solidification achieves near‐eutectic structure Fig. b . A small spherical primary Cr‐carbides are observed . vol. % in the eutectic matrix. Based on electron microprobe analysis EMPA , both coatings and contain Cr,Fe C primary and eutectic carbides. The Figure c shows a larger WC grains vol. % , which are embedded in the Ni‐Cr based matrix.
Abrasive wear tests are carried out on the scratch tester under the dry conditions, in ambient air at room temperature ≈ °C . A schematic diagram of scratch testing is presented in Figure . Stylus indenter was pressed with selected normal load , and N against surface of the test sample and moved with constant speed mm/s , producing the scratch of certain width and length mm on the test sample. )ndenter had Rockwell shape and the cone was diamond with radius of . mm.
Fig.2. Schematic diagram of scratch testing.
On surface of each material under investigation at least three scratches are made with a gap between scratches of at least mm. Before and after testing, both the indenter and the test samples are degreased and cleaned with benzene. The wear scar widths on the surface of the test samples are measured from SEM images at the end of testing. The wear scar widths and the known indenter geometry are used to
calculate the volume loss. After testing, the morphology of the test samples worn surfaces is examined with SEM.
The results of the wear tests are presented in Figures , and . Taking into account significant differences in structure homogeneity of the hardfaced coatings Fig. , the repeatability of the results, in terms of standard deviations, is satisfactory within % . Wear rate of the tested materials volume loss divided by scratch length increases with normal loading, as expected. The highest wear exhibits coating T. Nevertheless, wear rates for all coatings are high, even for abrasive wear. The reason for this is primarily due to the experimental conditions.
The test conditions were specific, i.e. the speeds were very low mm/s and the contact stresses very high. At the end of test, the normal stresses were between and GPa, which depends on the material, i.e. scratch width and applied normal load. With these conditions, a high‐stress or even gouging abrasion can be expected. With high‐stress abrasion, the worn surface may exhibit varying degrees of scratching with plastic flow of sufficiently ductile phases or fracture of brittle phases. )n gouging abrasion, the stresses are higher than those in high‐stress abrasion, and they are accompanied by large particles removal from the surface, leaving deep groves and/or pits [ ].
Coating 4541 (v = 4 mm/s)
0.0 0.4 0.8 1.2 1.6 2.0 2.4 2.8 3.2
10 50 100
Normal load, N
Fig. 3. Wear rates of coating for different normal loads.
Coating 5006 (v = 4 mm/s)
0.0 0.4 0.8 1.2 1.6 2.0 2.4 2.8 3.2
10 50 100
Normal load, N
Fig. 4. Wear rates of coating for different normal loads.
Coating 7888 T (v = 4 mm/s)
0.0 0.4 0.8 1.2 1.6 2.0 2.4 2.8 3.2
10 50 100
Normal load, N
Fig. 5. Wear rates of coating T for different normal loads.
0.00 0.50 1.00 1.50 2.00 2.50 3.00 3.50
670 690 710 730 750 770 790
10 N 50 N 100 N
Fig.6. Wear rate vs. hardness of tested materials for different normal loads.
For all applied loads, the relation between hardness and wear rate is non‐linear. )t is more curved for higher loads Fig. . This is connected with the coatings structure and exhibited wear mechanism. Coatings and exhibit mainly ploughing abrasive wear Fig. a , while coating T dominant type of abrasive wear is fracture cracking abrasive wear Fig. b .
Scratch test offers relatively easy and quick comparison of different materials on abrasive wear.
Structure of tested coatings showed influence on the dominant type of abrasive wear, which together with coatings hardness determined coatings abrasive wear resistance.
Coatings with lower hardness showed lower abrasive wear resistance, but the dependence
hardness vs. wear rate was non‐linear.
)n the case of iron‐based coatings, dominant type of abrasive wear was ploughing and in the case of WC‐based coatings, it was fracture
cracking abrasive wear.
This work has been performed as a part of activities within the projects TR , TR and TR . These projects are supported by the Republic of Serbia, Ministry of Education, Science and Technological Development, whose financial help is gratefully acknowledged.
[ ] A. Rac: Osnovi tribologije, Mašinski fakultet
Univerziteta u Beogradu, Beograd, .
[ ] R.G. Bayer: Fundamentals of wear failures, in: ASM Handbook Volume 11,Failure Analysis and Prevention, ASM )nternational, Metals Park, pp.
‐ , .
[ ] V. Lazić, M. Jovanović, D. Milosavljević, M. Mutavdžić, R. Čukić: Choosing of the most suitabletechnologyofhardfacingofmixerblades usedinasphaltbases, Tribology in )ndustry, Vol.
, No. ‐ , pp. ‐ , .
[ ] V. Lazić, M. Mutavdžić, D. Milosavljević, S. Aleksandrović, B. Nedeljković, P. Marinković, R. Čukić: Selectionofthemostappropriatetechnology of reparatory hard facing of working parts on universal construction machinery, Tribology in
)ndustry, Vol. , No. , pp. ‐ , .
[ ] J.R. Davis, Hardfacing, weld cladding, and dissimilar metal joining, in: ASM Handbook Volume 6,Welding,Brazing,andSoldering, ASM
)nternational, Metals Park, pp. ‐ , . [ ] EN : Welding consumables – Welding
consumables for hard‐facing, European
Committee for Standardization, Brussels, . [ ] M. Šolar, M. Bregant: Dodatnimaterijaliinjihova
upotreba kod reparaturnog navarivanja,
Zavarivanje i zavarene konstrukcije, Vol. , No. , pp. ‐ , .
[ ] A. Vencl, N. Manić, V. Popovic, M. Mrdak:
Possibility of the abrasive wear resistance determination with scratch tester, Tribology
Letters, Vol. , No. , pp. ‐ , .
[ ] B.R. Gligorijevic, A. Vencl, B.T. Katavic:
Characterizationandcomparisonofthecarbides morphologies in the near surface region of the single‐ and double layer iron‐based hardfaced coatings, Scientific Bulletin of the "Politehnica"
University of Timișoara, Transactions on Mechanics, Vol. , Special )ssue S , pp. ‐
[ ]OECD, Research Group on Wear of Engineering Materials, Glossary of Terms and Definitions in the Field of Friction, Wear and Lubrication: Ttribology, Organisation for Economic Co‐
operation and Development, Paris, . [ ]A. Vencl, A. Rac, B. )vković: Investigation of
abrasive wear resistance of ferrous‐based coatings with scratch tester, Tribology in
)ndustry, Vol. , No. ‐ , pp. ‐ , . [ ]A. Alil, B. Katavić, M. Ristić, D. Jovanović, M.
Prokolab, S. Budimir, M. Kočić: Structural and mechanical properties of different hard welded coatings for impact plate for ventilation mill,